1.1 The Volclay® Waterproofing System consists of products that are based on or
use sodium bentonite as the principle waterproofing component. The system is used as
a damp-proofing or waterproofing membrane below ground to protect basements and
other underground structures against water penetration and water vapour transmission
from the ground. The system is also used to waterproof plaza decks where they act as a
roof to spaces below.
1.2 The system is based on two membranes, Voltex® and Swelltite®, with other
accessory products completing the system.
Technical Assessments of
products for building and
No. 507 (2006)
Allco Agencies Ltd
5 Airborne Road
Tel: 09 448 1185
Fax: 09 448 1186 2.1 The Volclay® Waterproofing System has been appraised for use as:
• an external waterproof tanking membrane to in-situ concrete, precast concrete and
concrete masonry basement constructions subject to hydrostatic pressures of up to 2
bar (20 metres); and,
• a damp-proof membrane (DPM) to slab-on-ground and basement constructions
following the principles of NZBC Acceptable Solution E2/AS1; and,
• a waterproof membrane to plaza deck roof structures.
BRANZ Limited BRANZ Pty Ltd
Private Bag 50 908 P O Box 830 2.2 The Volclay® Waterproofing System must:
Porirua City Brookvale • be used adequately confined and protected against damage during construction and
New Zealand NSW 2100 in service; and,
Tel: +64 4 237 1170 Australia • not be used where ground water conductivity exceeds 2,500µS/cm (Refer Paragraph
Fax: +64 4 237 1171 Tel: +61 2 9938 6011 12.1).
www.branz.co.nz Fax: +61 2 9938 6911
2.3 All installations incorporating the Volclay® Waterproofing System must be
the subject of specific design. Building designers are responsible for the incorporation
of the system following the guidance details provided by Allco Agencies Ltd. The
designer must provide design and installation detailing within the contract documents.
2.4 The Volclay® Waterproofing System must be installed by Allco Agencies Ltd
Approved and Trained Applicators.
Readers are advised to check the validity of this Certificate by referring to the Valid Certificates listing on the BRANZ website, or by contacting BRANZ.
Building Regulations • Is granular Volclay® Bentonite used to detail areas that may
require additional Volclay® protection. It is supplied in 25 kg
New Zealand Building Code (NZBC) bags.
3.1 In the opinion of BRANZ, the Volclay® Volclay® Seamtape
Waterproofing System if designed, used, installed and • Is a tacky butyl rubber tape used to seal Swelltite® overlap
maintained in accordance with the statements and conditions seams and membrane edges from inclement weather and
of this Certificate, will meet the following provisions of the construction debris. It is supplied in 12.5 m long rolls.
NZBC: Volclay® M-2000 Liquid Flashing
Clause B2 DURABILITY: Performance B2.3.1 (a) not less
than 50 years. The Volclay® Waterproofing System meets this • Is trowel grade bitumen modified polyurethane
requirement. See Paragraph 14.1. waterproofing mastic used to detail around penetrations,
Clause E2 EXTERNAL MOISTURE: Performance E2.3.3. drains and at corner transitions. It is supplied in 7 litre tins.
The Volclay® Waterproofing System meets this requirement.
See Paragraphs 16.1 – 16.3.
Clause F2 HAZARDOUS BUILDING MATERIALS: Handling and Storage
Performance F2.3.1. The Volclay® Waterproofing System meets 5.1 Handling and storage of all materials whether on
this requirement and will not present a health hazard to people. or off site is under the control of the Approved and Trained
Applicator. Dry storage must be provided for all products and
3.2 This Certificate appraises the Volclay® Waterproofing the membranes must be protected from UV radiation.
System as an Alternative Solution in terms of New Zealand
Building Code compliance.
6.1 The Technical Literature which provides guidance for
Technical Specification designers is available from Allco Agencies Ltd.
4.1 Components and accessories for the Volclay®
Waterproofing System supplied by Allco Agencies Ltd are:
Voltex® Membrane Design Information
• Is a sheet membrane manufactured from two geotextile
membranes which are needle punched together and General
contain 5.3 kg/m2 of granular Sodium Bentonite. 7.1 Every installation of the Volclay® Waterproofing
The membrane bonds to poured concrete to form an System must be the subject of specific design. The designer is
integral seal in the form of a tenacious bond to prevent responsible for incorporating all design and installation details
water migration. The Voltex® membrane is supplied in within the construction documentation based on the guidance
1.2 m wide x 4.5 m long and 1.5 m wide x 40 m long rolls. documents provided by Allco Agencies Ltd.
• Is a sheet membrane made up of a blend of Sodium Bentonite
and Butyl Rubber integrally bonded between geomembrane Substrate Design
and a clear poly-siliconised release liner. It is used primarily 8.1 Substrate design must be in accordance with the
for waterproofing foundation walls and plaza roof decks. NZBC to relevant standards, such as, NZS 4203 for design
The Swelltite® membrane is supplied in a 1 m wide x 11.6 m loadings, NZS 3101 for insitu or precast concrete and NZS
long roll. 4210, 4229 and 4230 for concrete masonry.
Waterstop RX® 8.2 Soil substrates must be prepared in accordance with
the requirements of Allco Agencies Ltd. In general a minimum
• Is a flexible strip waterstop manufactured from 75% Sodium requirement is well-levelled soils without voids and debris,
Bentonite and 25% Butyl Rubber. It is primarily designed compacted to a minimum of 85% Modified Proctor density for
to stop water infiltration through both vertical and horizontal uniform support.
concrete construction joints, junctions between new and 8.3 The substrate must be solid and have a surface finish
existing construction, irregular surfaces and around wall that is smooth, clean and free from defects or irregularities
penetrations such as plumbing and electrical conduits. It is which may damage the membrane.
supplied in 10.2 m and 6.1 m long rolls. 8.4 The membrane must be confined to ensure a
WB-Adhesive™ watertight seal is achieved and maintained. For specific
• Is a non-flammable, latex, water based adhesive used to installation details refer to the Technical Literature or Allco
temporarily secure Waterstop RX® to concrete, metal, wood Agencies Ltd.
and PVC surfaces in vertical and horizontal applications. It 8.5 The Volclay® Waterproofing System may be used as
is packed in 1US Gallon cans. an alternative DPM material to the materials listed in NZBC
Bentoseal® Acceptable Solution E2/AS1, Section 12.
• Is a trowel grade sodium bentonite compound used as
detailing mastic around penetrations and corner transitions. Control Joints
It is supplied in US 3 Gallon pails. 9.1 Where control or construction joints are formed in the
Aquadrain® substrate, Allco Agencies Ltd must be consulted regarding the
• Is a prefabricated drainage composite consisting of a heavy use of the membranes over these joints.
filter fabric adhered to a high strength plastic drainage core.
It is supplied in 1.2 m wide x 15.6 m long rolls.
Backfilling and Drainage edge seal and protection, the backfill capping, subsoil drainage
10.1 Voltex and Swelltite membranes must be confined
® ® system and plaza deck finishing ensuring all are functioning as
and protected against damage. It is recommended that originally designed.
Aquadrain® is placed between the membrane and the granular 15.2 If required, the drainage system must be cleared to
fill. remove any sediment or silt build-up. The slope of the backfill
10.2 Backfilling should be undertaken as soon as possible capping must be maintained at all times.
after placing the Volclay® Waterproofing System. Swelltite®
must be backfilled the same day or whenever rain is imminent.
Exposed laps must be protected from the weather and External Moisture
termination bars must be sealed with an approved sealant. 16.1 The Volclay® Waterproofing System, when installed in
10.3 When being used as a DPM, backfilling, drainage accordance with this Certificate, will provide an effective barrier
and the backfill capping must be completed in accordance to liquid water and water vapour penetrating to the interior face
with NZBC Acceptable Solution E2/AS1, Paragraphs 12.3 and of basement retaining walls, floors and plaza roof decks.
12.3.1 and Figure 133. 16.2 The membranes have a vapour flow resistance of not
10.4 When being used as tanking membrane the backfill less than 90 MN s/g as required by NZBC Acceptable Solution
material must be free from builders debris and angular E2/AS1, Paragraph 12.2.1 (a).
aggregate and must be compacted to 85% Modified Proctor. 16.3 The system forms sealed joints and seals at
Further advice regarding backfilling is available from Allco penetrations.
Agencies Ltd. 16.4 Building designers must ensure junctions with other
10.5 After backfilling in either situation, the installation membranes, such as at the floor/wall junction, form a waterproof
is completed with a flashing in accordance with the details joint. Junctions with other membranes have not been assessed
contained within the Technical Literature to protect the upper and are outside the scope of this Certificate.
edge of the membrane.
Plaza Roof Deck
11.1 The Swelltite® membrane using Volclay® seamtapes to
seal Swelltite® over the lap joints is laid directly over reinforced Installation Skill Level Requirement
concrete plaza roof deck slabs. Aquadrain® drainage composite 17.1 Installation of the membranes must be completed by
is then laid fabric side up over the Swelltite® membrane. The Allco Agencies Ltd Approved and Trained applicators that have
Swelltite® system is then covered and protected by a minimum a minimum 3 years waterproofing application experience.
of 75 mm thick concrete wearing slab or clay, concrete or stone 17.2 Substrates must be completed by tradespersons skilled
pavers at least 50 mm thick laid on a bed of sand or cementitious in the relevant construction method chosen and in accordance
grout. For system details contact Allco Agencies Ltd. with instructions given within the Allco Agencies Ltd Technical
Literature and this Certificate.
12.1 The gelling of sodium bentonite is adversely affected System Installation
by the presence of electrolytes (particularly trivalent ions). Substrate Preparation
Calcium bentonite may be formed in hard waters and has inferior
18.1 All substrate surfaces must be checked to ensure they
gelling properties. Therefore if there are any concerns regarding
are clean, smooth and free from sharp edges, loose or foreign
ground water contamination (salinity), Allco Agencies Ltd offer
materials, oil, grease or other deleterious material that may
conductivity tests on soil water, and from these tests make a
damage the waterproofing membrane. Horizontal surfaces must
recommendation on the appropriate system specification. One
be free from standing water.
solution to contaminated area treatment is outlined in Paragraph
18.6. The membrane is not affected by organic contaminants. Membrane Installation
18.2 Voltex® is installed with the darker coloured face in
direct contact with the substrate to be waterproofed. Swelltite® is
Resistance to Loading installed with the sodium bentonite compound in direct contact
13.1 Providing Voltex® membranes are adequately with the substrate to be waterproofed. In the case of Swelltite®,
confined, properly hydrated, and not subject to point loading, sodium bentonite is exposed by removing the clear siliconized
an installation beneath a foundation slab will transmit dead and release sheet and side laps overlapped by a minimum of 50 mm
imposed loads safely without excessive deformation. and ends of sheets a minimum of 300 mm. Internal corners must
be reinforced with an 18 mm thick bead of Bentoseal.
18.3 Sealing around penetrations through the membrane,
Durability such as pile caps, service pipes and wall penetrations is
Serviceable Life performed by cutting a hole in the membrane, fitting it around
the penetration and detailing with an 18 mm cant of Bentoseal
14.1 The Volclay® Waterproofing System when used as a
or a paste made up insitu by mixing Bentonite granules with
tanking, waterproofing and DPM material is expected to have a
serviceable life of at least 50 years provided it is installed and
18.4 Termination bars and any exposed laps must be
maintained in accordance with this Certificate and is continually
temporarily sealed until the finished ground level is determined.
confined and protected from UV radiation and physical
The membrane should not finish above the finished ground level
and must be completed with a flashing or other technique as
shown in the Technical Literature.
18.5 Aquadrain® must be installed before backfilling.
Maintenance Backfilling must commence immediately after the membrane
15.1 Annual inspections must be made of the membrane top
is installed to ensure the membrane is confined correctly. responsibility of Allco Agencies Ltd.
Compact backfill, approved by Allco Agencies Ltd, in 22.4 Quality of installation on site is the responsibility
300-400 mm lifts compacted to 85% Modified Proctor of the installer.
density. With plaza roof decks the Aquadrain® is used under 22.5 Building contractors are responsible for the quality
an approved wear layer system. Contact Allco Agencies of construction of substrate systems in accordance with the
Ltd for “Technical Reference 205” a full specification on instructions of Allco Agencies Ltd.
backfilling requirements and approved wear layer systems. 22.6 Designers are responsible for the building design
18.6 In chemically contaminated areas the membrane and the design and installation details for the Volclay®
can be pre-hydrated by deliberately soaking with clean, Waterproofing System.
cold mains water and leaving to soak for 2-3 hours before 22.7 Building owners are responsible for the
backfilling or pouring the concrete. maintenance of the top edge of the membrane system and
Inspections plaza deck finishes in accordance with the instructions of
Allco Agencies Ltd.
18.7 The contract documents must be referred to during
the inspection of substrate and membrane installations by
building consent authorities and territorial authorities.
Sources of Information
• British Board of Agrément Certificate No. 86/1650,
Volclay® Waterproofing System for Structures.
Health and Safety • NZS 3101: 1995 The design of concrete structures.
19.1 Safe use and handling procedures for the
• NZS 3604: 1999 Timber framed buildings.
membrane system are provided in the Technical Literature.
• NZS 4203: 1992 General structural design and design
loadings for buildings.
• NZS 4210: 1989 Masonry construction: Materials and
Basis of Appraisal Workmanship.
• NZS 4229: 1999 Concrete masonry buildings not
The following is a summary of the technical investigations requiring specific engineering design.
carried out: • NZS 4230: 2004 Design of reinforced concrete masonry
Tests • Compliance Document for New Zealand Building Code
20.1 The following is a summary of the supplied testing External Moisture Clause E2, Department of Building
information on Volclay® Waterproofing System: and Housing, Third Edition July 2005.
• Hydraulic Conductivity Determination to ASTM D- • New Zealand Building Code Handbook and Approved
5084. Documents, Building Industry Authority, 1992.
• Low Temperature Flexibility to ASTM D 1970 • The Building Regulations 1992, up to, and including
• Tensile Strength to ASTM D 4632 October 2004 Amendment.
• Puncture Resistance to ASTM D 4833.
• Concrete adhesion to ASTM D 903
• Hydrostatic pressure resistance to ASTM D 5385
• An investigation of the effectiveness of Voltex® as a
Water Vapour Barrier by University of Hertfordshire.
Test methods and results have been reviewed by BRANZ
and found to be satisfactory.
20.2 The Volclay® Waterproofing System has held a
valid BBA Agrément Certificate (UK) since 1986.
21.1 A durability opinion has been given by BRANZ
21.2 Practicability of installation has been assessed by
BRANZ and found to be satisfactory.
21.3 The Technical Literature has been examined
by BRANZ and found to provide satisfactory guidance
to designers for the use of the Volclay® Waterproofing
22.1 The manufacture of the membranes and primer has
not been examined by BRANZ, but details regarding the
quality and composition of the materials used were obtained
by BRANZ and found to be satisfactory.
22.2 The quality management system of the membrane
manufacturer, Cetco Building Materials Group, USA has
been assessed and accredited as meeting the requirements of
BS EN ISO 9001: 2000 by BSI Management Systems, USA,
Registration Number FM 67591.
22.3 The quality of materials supplied is the
In the opinion of BRANZ, the
Volclay® Waterproofing System
is fit for purpose and will comply
with the Building Code to the
extent specified in this Certificate
provided it is used, designed,
installed and maintained as set out
in this Certificate.
The Appraisal Certificate is issued
only to the Certificate Holder,
Allco Agencies Ltd, and is valid
until further notice, subject to the
Conditions of Certification.
Conditions of Certification
1. This Certificate:
a) relates only to the product as described
b) must be read, considered and used in full
together with the technical literature;
c) does not address any Legislation, Regulations,
Codes or Standards, not specifically named
d) is copyright of BRANZ.
2. The Certificate Holder:
a) continues to have the product reviewed by
b) shall notify BRANZ of any changes in
product specification or quality assurance
measures prior to the product being
c) abides by the BRANZ Appraisals Services
Terms and Conditions.
3. The product and the manufacture are
maintained at or above the standards, levels
and quality assessed and found satisfactory
4. BRANZ makes no representation as to:
a) the nature of individual examples of, batches
of, or individual installations of the product,
including methods and workmanship;
b) the presence or absence of any patent or
similar rights subsisting in the product or any
c) any guarantee or warranty offered by the
5. Any reference in this Certificate to any other
publication shall be read as a reference to the
version of the publication specified in this
Date of issue: 11 April 2006